**Louisiana State University**

**LSU Digital Commons**

LSU Doctoral Dissertations Graduate School

2010

### Carbon Nanotube Interconnect Modeling for Very

### Large Scale Integrated Circuits

Yao Xu

*Louisiana State University and Agricultural and Mechanical College*

Follow this and additional works at:https://digitalcommons.lsu.edu/gradschool_dissertations Part of theElectrical and Computer Engineering Commons

This Dissertation is brought to you for free and open access by the Graduate School at LSU Digital Commons. It has been accepted for inclusion in LSU Doctoral Dissertations by an authorized graduate school editor of LSU Digital Commons. For more information, please contactgradetd@lsu.edu.

Recommended Citation

*Xu, Yao, "Carbon Nanotube Interconnect Modeling for Very Large Scale Integrated Circuits" (2010). LSU Doctoral Dissertations. 3778.*
https://digitalcommons.lsu.edu/gradschool_dissertations/3778

**CARBONNANOTUBEINTERCONNECTMODELINGFORVERYLARGE**

**SCALEINTERGRATEDCIRCUITS **

A Dissertation

Submitted to the Graduate Faculty of the Louisiana State University and Agricultural and Mechanical College

in Partial fulfillment of the requirements for the degree of

Doctor of Philosophy

in

The Department of Electrical and Computer Engineering

by

Yao Xu

B.S., Tsinghua University, Beijing, China July, 2000

M.S., Louisiana State University, Baton Rouge, LA 70803, USA May, 2011

**To my loving and supportive wife, Xiuli **

**To my loving and supportive wife, Xiuli**

**& **

**&**

**ACKOWLEDGMENTS **

My thanks and special appreciation to my advisor and mentor Dr. Ashok Srivastava. I am very thankful for his guidance, patience and understanding throughout my dissertation research. I would have not completed this research without his suggestions, discussions and constant encouragement.

I would like to thank Committee members Late Dr. Jorge L. Aravena, Dr. Tryfon T. Charalampopoulos, Dr. Jin-Woo Choi, Dr. Theda Daniels-Race, Dr. Jonathan P. Dowling, Dr. Martin Feldman, Dr. Suresh Rai and Dr. R. Vaidyanathan for being a part of my committee.

I am thankful to Dr. Ashwani K. Sharma of US Air Force Research Laboratory, Kirtland Air Force Base, New Mexico, for his support and encouragement for the research carried out in this project.

Above all, I am deeply grateful to my fellow co-workers, Chen Fang, Yang Liu, Chunbo Ni, Dr. Jose Mauricio Marulanda Prado, Wei Shu, Rajiv Soundararajan, Juyu Wang and Dr. Siva Yellampalli.

**TABLE OF CONTENTS **

ACKNOWLEDGMENTS ... iii

LIST OF TABLES ... vi

LIST OF FIGURES ... vii

ABSTRACT………. ... xiii

CHAPTER 1 INTRODUCTION ... 1

1.1 Challenges of Silicon Integrated Circuits ... 1

1.2 Introduction to Carbon Nanotubes ... 1

1.3 Structure of Carbon Nanotubes ... 2

1.4 Properties of Single-Walled Carbon Nanotubes ... 5

1.4.1 Electronic Band Structure ... 6

1.4.2 Density of States ... 10

1.5 Applications of CNTs in Integrated Circuits ... 14

1.5.1 Applications of Semiconducting Carbon Nanotubes ... 14

1.5.2 Applications of Metallic Carbon Nanotubes ... 15

1.6 Synthesis of Carbon Nanotubes ... 16

1.7 CNT Based Circuit Modeling ... 18

1.7.1 CNT-FET Modeling ... 18

1.7.2 CNT Interconnect Modeling ... 19

1.8 Scope of Research ... 19

CHAPTER 2 CARBON NANOTUBE FIELD-EFFECT TRANSISTOR ... 21

2.1 Background of CNT-FETs ... 21

2.2 Surface Potential of CNT-FETs ... 25

2.3 Non-Ballistic CNT-FET Modeling ... 36

2.3.1 Current Transport Modeling ... 36

2.3.2 Logic Gates Modeling ... 37

2.3.3 Dynamic Modeling ... 42

2.4 Ballistic CNT-FET Modeling ... 48

2.5 Verilog-AMS Simulations ... 50

2.6 Summary ... 53

CHAPTER 3 MODELING SINGLE-WALLED CARBON NANOTUBE INTERCONNECTION FOR VLSI ... 59

3.1 Introduction to Carbon Nanotube Interconnection ... 59

3.2 Two-Dimensional Fluid Model... 61

3.3 One-Dimensional Fluid Model ... 65

3.4 Transmission Line Model ... 71

3.5 Results and Discussion ... 73

CHAPTER 4 MODELING MULTI-WALLED AND BUNDLE OF

SINGLE-WALLED CARBON NANOTUBES INTERCONNECTION FOR

VLSI ... 88

4.1 MWCNT Interconnection Modeling ... 88

4.2 SWCNT Bundle Interconnection Modeling ... 91

4.3 Performance of MWCNT and Bundles of SWCNT Interconnects ... 96

4.4 Summary ... 110

CHAPTER 5 CARBON NANOTUBE WIRE INDUCTOR ... 111

5.1 On-Chip Inductor Modeling ... 112

5.2 LC Voltage-Controlled Oscillator (VCO) ... 114

5.3 Summary ... 122

CHAPTER 6 ENERGY RECOVERY TECHNIQUES ... 123

6.1 Energy Recovery Logic (ERL) ... 124

6.1.1 2N-2N2P Logic ... 124

6.1.2 Quasi-Static Energy Recovery Logic (QSERL) ... 126

6.1.3 Clocked Adiabatic Logic (CAL) ... 128

6.1.4 New CAL XNOR/XOR Gate ... 128

6.1.5 Simulation Results ... 131

6.1.6 Experimental Results ... 135

6.2 CNT-FET Energy Recovery Circuits ... 135

6.3 Summary ... 140

CHAPTER 7 FAULT MODELING IN CNT BASED DIGITAL CIRCUITS ... 141

7.1 CNT-FET Logic Gates ... 141

7.2 Fault Models ... 144

7.2.1 Stuck-At Fault Model ... 144

7.2.2 Stuck-Open Fault Model ... 144

7.2.3 Stuck-On Fault Model ... 144

7.3 Summary ... 146

CHAPTER 8 CONCLUSION AND SCOPE OF FUTURE WORK ... 149

8.1 Conclusion ... 149

8.2 Scope of Future Work ... 151

REFERENCES……… ... 153

APPENDIX A VERILOG-AMS CODES FOR NONBALLISTIC CNT-FET MODELING ... 173

APPENDIX B CARBON NANOTUBE FOR BIO- AND CHEMICAL SENSING ... 180

**LIST OF TABLES **

Table 1.1: Mechanical properties of carbon nanotubes and

comparison with other materials [27] ... 4

Table 1.2: Electrical properties of carbon nanotubes and comparison

with other materials [28, 29] ... 4

Table 4.1: A comparison of calculated and measured resistances of

MWCNT interconnects ... 100

Table 4.2: A comparison of MWCNT interconnect model parameters ... 100

Table 4.3: Power dissipation ratio of MWCNT and SWCNT bundle

**LIST OF FIGURES **

Figure 1.1: Single-walled carbon nanotube (Nanotube Modeler

Software) [26]. ... 3

Figure 1.2: Multi-walled carbon nanotubes (Nanotube Modeler

Software) [26]. ... 3

Figure 1.3: Single-walled carbon nanotubes bundle (Nanotube

Modeler Software) [26]. ... 3

Figure 1.4: Schematic representation of a chiral vector in the crystal

lattice of a carbon nanotube. ... 7

Figure 1.5: Schematic representation of (a) crystal lattice and (b)

reciprocal lattice of a carbon nanotube with chiral vector

(4,3). ... 9

Figure 1.6: Plot of the allowed wave vectors in k-space for a CNT

with (a) chiral vector (4,2) and (b) chiral vector (8,2). ... 11

Figure 1.7: Plot of the energy band diagram in k-space for a CNT with

**(a) chiral vector (4,2) and (b) chiral vector (8,2). Note: **
Bang gap is the distance between the top of the valence
band and the bottom of the conduction band marked by 1

in (a). ... 12

Figure 1.8: Plot of the density of states for a CNT with (a) chiral

vector (4,2) and (b) chiral vector (8,2). ... 13

Figure 2.1: **Typical vertical cross-section of a CNT-FET. Note: **

Insulators in the figure are SiO2 or high-κ dielectric. ... 24 Figure 2.2: (a) Plot of the charges from the gate to the substrate for

Schottky Barrier CNT-FET, (b) Plot of the charges from the gate to the substrate for MOSFET-like CNT-FET and (c) plot of the potential distribution from the gate to the

substrate in a CNT-FET [91]. ... 26

Figure 2.3: Energy band diagram of a two terminal CNT-FET for (a)

Vgb = Vfb and (b) Vgb > 0. Note: HfO2 is the high-κ

dielectric hafnium oxide [91]. ... 32

Figure 2.5: Current, Ids versus gate to source voltage, Vgs using Vfb = -0.79 and ф0 =0 for CNT-FET (11,9). The device dimensions are: Tox1 = 15 nm, Tox2 = 120 nm and L = 250

nm. In modeled curve, Q01 = Q02 = 0 and λ = 0.1 V-1. ... 39 Figure 2.6: CNT-FET logic: (a) Inverter, (b) two input NAND gate

and (c) two input NOR gate. ... 40

Figure 2.7: Voltage transfer characteristics of an inverter using

CNT-FETs (11,9) with Vfb = 0 V, λ = 0, 0.1 V-1 and ф0 = 0. The dimensions of both the n-type FET and p-type

CNT-FET are: Tox1 = 15 nm, Tox2 = 120 nm and L = 250 nm. ... 41 Figure 2.8: Voltage transfer characteristics of (a) an inverter and a

NAND gate (b) an inverter and a NOR gate using CNT-FETs (11,9) with Vfb = 0 V and ф0 = 0. The dimensions of both the n-type CNT-FET and p-type CNT-FET are: Tox1

= 15 nm, Tox2 = 120 nm and L = 250 nm. ... 43 Figure 2.9: Meyer capacitance model for CNT-FETs [114]. ... 44

Figure 2.10: The capacitances of CNT-FET (11,9) with Vfb = -0.79 V and ф0 = 0. The device dimensions are Tox1 = 15 nm, Tox2 = 120 nm and L = 250 nm. In modeled curve, Q01 = Q02 =

0. ... 49

Figure 2.11: I-V characteristics for a self-aligned p-type CNT-FET

with Ohmic metallic contacts shown by solid lines. The CNT-FET parameters are: κ = 15, tox = 8 nm and d = 1.7nm. Experimental data shown by rectangles is taken from the work of Javey et al. [49]. Dotted line plots are

from the work of Akinwande et al. [116] ... 51

Figure 2.12: I-V characteristics of ballistic CNT-FET (19,5) for

different numbers of sub-bands. ... 52

Figure 2.13: Steps to simulate a new device using Verilog-AMS code. ... 54

Figure 2.14: (a) Transient behavior of an inverter pair using CNT-FETs

(11,9) with Vfb = 0 V and ф0 = 0. The dimensions of both the n-type CNT-FET and p-type CNT-FET are: Tox1 = 15 nm, Tox2 = 120 nm and L = 250 nm and (b) average delay

of the inverter pair versus supply voltage. ... 55

Figure 2.15: (a) Schematic of a 5-stage ring oscillator, (b) output

waveform, (c) the oscillating frequency versus supply voltage, VDD. The dimensions of both the n-type and

Figure 2.16: Oscillating frequency of the 5-stage ring oscillator versus

length of the CNT-FETs. ... 57

Figure 3.1: Geometry of a single wall carbon nanotube (SWCNT). ... 63

Figure 3.2: The equivalent circuit of a metallic SWCNT interconnect. ... 74

Figure 3.3: Equivalent circuit of a SWCNT contact. ... 74

Figure 3.4: │Zin│ versus frequency for different lengths of SWCNTs. ... 76

Figure 3.5: │Zin│ versus frequency using different model for a 10 µm length SWCNT. ... 77

Figure 3.6: Schematic of a 2-port network of interconnects. ... 79

Figure 3.7: S21 (amplitude) versus frequency for different lengths SWCNT and Cu interconnects. ... 81

Figure 3.8: S11 (amplitude) versus frequency for different lengths SWCNT and Cu interconnects. ... 82

Figure 3.9: S21 (amplitude) versus frequency using different model for a 1 µm length SWCNT. ... 83

Figure 3.10: S11 (amplitude) versus frequency using different model for a 1 µm length SWCNT. ... 84

Figure 3.11: Group delay versus frequency for different lengths SWCNT and Cu interconnects. ... 87

Figure 4.1: Equivalent circuit of a metallic MWCNT interconnect. ... 92

Figure 4.2: Simplified equivalent circuit of a metallic MWCNT interconnect. ... 92

Figure 4.3: Simple equivalent circuit model of a metallic MWCNT interconnect. ... 92

Figure 4.4: Cross-section of a SWCNT bundle interconnect. ... 94

Figure 4.7: Comparison of S21 from our model and Li et al. model [181] for MWCNT interconnects: (a) amplitude and (b)

phase. ... 101

Figure 4.8: Comparison of S11 from our model and Li et al. model [181] for MWCNT interconnects: (a) amplitude and (b)

phase. ... 102

Figure 4.9: Calculated S-parameters of different interconnects: (a) S21

(amplitude) and (b) S11 (amplitude). ... 104 Figure 4.10: Inverter pair with interconnects. ... 106

Figure 4.11: Output waveforms of an inverter pair with 10 μm length

of different interconnect wires. ... 107

Figure 4.12: Propagation delays of interconnects of different lengths

for 22 nm technology. ... 108

Figure 5.1: π model of an on-chip inductor. ... 113

Figure 5.2: Q-factor of inductors based on CNT and Cu. ... 115

Figure 5.3: (a) Circuit diagram of a CMOS cross-coupled LC VCO,

(b) equivalent circuit of LC VCO and (c) circuit to

estimate the negative resistance of the cross-coupled pair. ... 117

Figure 5.4: C-V curve of a varactor. ... 118

Figure 5.5: VCO oscillation frequency versus control voltage with

difference inductors. ... 120

Figure 5.6: VCO phase noise versus offset frequency. ... 121

Figure 6.1: (a) CMOS circuit of 2N-2N2P XNOR/XOR gate and (b)

timing for 2N-2N2P XNOR/XOR. ... 125

Figure 6.2: (a) Quasi-static energy recovery logic (QSERL), (b)

Complementary clocked power supplies, (c) CMOS circuit of QSERL XNOR/XOR gate and (d) separated

QSERL XNOR and XOR gates. ... 127

Figure 6.3: (a) CMOS circuit of CAL XNOR/XOR gate and (b)

idealized CAL timing waveforms. ... 129

Figure 6.4: (a) CMOS circuit of new CAL XNOR/XOR gate and (b)

ideal new CAL input waveforms. Note: XOR(O/P) =

Figure 6.5: Simulated New CAL waveforms. ... 132

Figure 6.6: Simulated energy dissipation of different ERL

XNOR/XOR gates. ... 133

Figure 6.7: Simulated power dissipation versus frequency. ... 134

Figure 6.8: (a) Microphotograph of CAL XNOR/XOR gates and (b)

experimental results. ... 136

Figure 6.9: Average power density for a CNT-FET inverter. Note:

The plot is obtained from Verilog-AMS in

Cadence/Spectre. ... 137

Figure 6.10: CNT-FET New CAL XNOR/XOR. Note: XOR(O/P) =

AB+ AB and XNOR(O/P) = AB+ A B. ... 138

Figure 6.11: Average power density of different CNT-FET

XNOR/XOR energy recovery circuits. ... 139

Figure 7.1: (a) CNT-FET inverter and (b) of CNT-FET inverter layout

[44]. ... 142

Figure 7.2: (a) CNT-FET NAND and NOR gates and (b) of CNT-FET

NAND and NOR gates layouts. ... 143

Figure 7.3: (a) Physical layout showing shorts in a CNT-FET NAND

gate with stuck-at faults (dotted lines) and (b) open faults

shown by X in the circuit. ... 145

Figure 7.4: Transient simulations of a 2-input CNT-FET NAND gate

with and without stuck-at faults. ... 147

Figure 7.5: Transient simulations of a 2-input CNT-FET NAND gate

with and without stuck-open faults. ... 148

Figure B.1: Transient behavior of an inverter pair inter-connected by

100μm CNT wire length before and after SOCl2

adsorption. ... 181

Figure B.2: RO frequency dependence on supply voltage, VDD. The dimensions of both the n-type and p-type CNT-FETs are:

Figure C.2: Top-view of MWCNT interconnects between electrodes

(unit: µm). ... 183

Figure C.3: Top-view of the mask for first lithography step. ... 185

Figure C.4: Top-view of the structure after the first lithography step

and metal etching. ... 186

Figure C.5: Cross-section of the structure after the first lithography

step and metal etching. ... 187

Figure C.6: Cross-section of the structure after MWCNTs are aligned

between electrodes. ... 187

Figure C.7: Top-view of the structure after second lithography step. ... 188

Figure C.8: Cross-section of the structure after second metal

deposition (Au). ... 189

**ABSTRACT **

In this research, we have studied and analyzed the physical and electrical properties of carbon nanotubes. Based on the reported models for current transport behavior in non-ballistic CNT-FETs, we have built a dynamic model for non-ballistic FETs. We have also extended the surface potential model of a non-ballistic FET to a ballistic FET and developed a current transport model for ballistic CNT-FETs.

We have studied the current transport in metallic carbon nanotubes. By considering the electron-electron interactions, we have modified two-dimensional fluid model for electron transport to build a semi-classical one-dimensional fluid model to describe the electron transport in carbon nanotubes, which is regarded as one-dimensional system. Besides its accuracy compared with two-dimensional fluid model and Lüttinger liquid theory, one-dimensional fluid model is simple in mathematical modeling and easier to extend for electronic transport modeling of multi-walled carbon nanotubes and single-walled carbon nanotube bundles as interconnections.

Based on our reported one-dimensional fluid model, we have calculated the parameters of the transmission line model for the interconnection wires made of single-walled carbon nanotube, multi-single-walled carbon nanotube and single-single-walled carbon nanotube bundle. The parameters calculated from these models show close agreements with experiments and other proposed models. We have also implemented these models to study carbon nanotube for on-chip wire inductors and it application in design of LC voltage-controlled oscillators.

By using these CNT-FET models and CNT interconnects models, we have studied the behavior of CNT based integrated circuits, such as the inverter, ring oscillator, energy recovery logic; and faults in CNT based circuits.

**CHAPTER 1 **

**1 **

**INTRODUCTION **

**1.1 Challenges of Silicon Integrated Circuits **

Semiconductor Research Corporation (SRC) in its International Technology Roadmap of Semiconductors report (ITRS 2003) has refereed to several non-classical devices, which could be the candidates of future technology to replace the existing silicon MOSFETs as the end of Moore’s law approaches year 2020 [1]. Double gate MOSFET and FinFET are recognized as two of the most promising candidates for future very large scale integrated (VLSI) circuits [2-5]. The carbon nanotube field-effect transistor (CNT-FET) is regarded as an important contending device to replace silicon transistors [6, 7] since many of the problems that silicon technology is facing are not present in CNTs. For example, carrier transport is 1-D in carbon nanotubes; the strong covalent bonding gives the CNTs high mechanical and thermal stability and resistance to electromigration; and diameter is controlled by its chemistry and not by the standard conventional fabrication process [2].

For interconnects, as CMOS processes scale into the nanometer regime, lithography limitations, electromigration, and the increasing resistivity and delay of copper interconnects have driven the need to find alternative interconnect solutions [8]. Carbon nanotubes have emerged as a potential candidate to supplement copper interconnects because of their ballistic transport and ability to carry large current densities in the absence of electromigration [9]. Previous studies that assess the potential use of CNTs as interconnects [10-13] primarily focus on the relative interconnect delay of CNTs to copper for sub-nm CMOS technology nodes. Carbon nanotubes are being explored extensively as the material for making future complementary devices, integrated circuits [14-16], interconnects [17] and hybrid CMOS/Nanoelectronic circuits [18].

**1.2 Introduction to Carbon Nanotubes **

In 1991, electron microscopist Sumio Iijima [19], of the NEC laboratories in Japan discovered the carbon nanotubes that are a tubular shape in the form of coaxial tubes of graphitic sheets, ranging from two shells to approximately fifty. These structures

were categorized as the multi-walled carbon nanotubes (MWCNTs). Subsequently growth of single-walled carbon nanotubes (SWCNTs) were reported by Bethune et al. [20] and Iijima and Ichihashi [21].

Most SWCNTs have a diameter close to 1 nanometer, with a tube length that can be many thousands of times longer. The structure of a SWCNT can be conceptualized by wrapping an atomic thick layer of graphite called graphene into a seamless cylinder. Multi-walled carbon nanotubes consist of multiple layers of graphite rolled in to form a tubular shape. Since CNTs are planar graphite sheets wrapped into tubes, electrical characteristics vary with the tube diameter and the wrapping angle of graphene [22]. One of the interesting features of the carbon nanotube is that it can be metallic or semiconducting with bandgap depending on its chirality [23-25]. In the following, we discuss structure and electronic behavior of carbon nanotubes.

**1.3 Structure of Carbon Nanotubes **

There are four types of natural occurring carbon, diamond, graphite, ceraphite, and fullerenes. Fullerenes are molecules formed entirely of carbon and take the shape of a hollow sphere, ellipsoid, or a tube. Fullerenes that take the shape of a tube are called buckytubes or nanotubes.

Carbon nanotubes can be pictured as a result of folding graphene layers into a tubular structure as seen in Fig. 1.1 [26]. These cylindrical form of carbon nanotubes can be single-walled or multi-walled depending on the number of shells that form the tubular structure [25]. Single-walled carbon nanotubes are composed of one shell of carbon atoms. Multi-walled carbon nanotubes have multiple nested shells of carbon atoms, as shown in Fig. 1.2. Single-walled carbon nanotubes tend to adhere strongly to each other forming ropes or bundles of nanotubes as shown in Fig. 1.3 [26] exhibiting physical properties of both metallic and semiconducting materials [22].

Figure 1.1: Single-walled carbon nanotube (Nanotube Modeler Software) [26].

Figure 1.2: Multi-walled carbon nanotubes (Nanotube Modeler Software) [26].

Table 1.1: Mechanical properties of carbon nanotubes and comparison with other
materials [27]
**Material **
**Young's **
**Modulus **
**(TPa) **
**Tensile **
**Strength **
**(GPa) **
**Elongation at **
**Break (%) **
**Thermal **
**Conductivity **
**(W/mK) **
**SWCNT ** 1-5 13-53 16 3,500-6,600
**MWCNT ** 0.27-0.95 11-150 8.04-10.46 3000
**Stainless **
**steel ** 0.186-0.214 0.38–1.55 15-50 16
**Kevlar ** 0.06–0.18 3.6–3.8 ~2 ~1
**Copper ** 0.11–0.128 0.22 385
**Silicon ** 0.185 7 149

Table 1.2: Electrical properties of carbon nanotubes and comparison with other materials [28, 29]

**Semiconductor Metal **

**Parameter ** **Semiconducting _{SWCNT }**

**Silicon GaAs**

**Ge Parameter**

_{SWCNT }Metallic**Copper**

**Bandgap **
**(eV) ** 0.9/diameter 1.12 1.424 0.66
**Mean **
**Free Path **
**(nm) **
1,000 40
**Electron **
**Mobility **
**(cm2/Vs) **
20,000 1,500 8,500 3,900 **Current density **
**(A/cm2) **
1010 106
**Electron **
**Phonon **
**Mean **
**Free **
**Path (Å) **
~700 76 58 105
**Resistivity**
**(Ω·m) **
~10-5 1.68×10−8

Metallic carbon nanotubes conduct extremely large amount of current densities. This property is what allows the application of metallic CNTs in interconnection substituting to metal wires, such as Cu, for the next generation of integrated circuits. On the other hand, semiconducting CNTs can be switched on and off by using a gate electrode. This property is what allows the application of CNTs in implementing field-effect transistors.

Single-walled carbon nanotubes have risen as one of the most likely candidates for miniaturizing electronics beyond current technology. The most fundamental application of metallic SWCNTs is in interconnection. Since it is difficult to prepare metallic CNT, fabrication and process integration of MWCNTs and CNT bundles interconnects have been reported [30, 31]. This work will focus on carbon nanotube field-effect transistors (CNT-FETs) and CNT interconnects made using semiconducting and metallic single-walled carbon nanotubes (SWCNTs), respectively, and on some basic circuits, such as the inverter and ring oscillator which are composed of complementary CNT-FETs and CNT interconnects.

**1.4 Properties of Single-Walled Carbon Nanotubes **

Single-walled carbon nanotubes can be characterized by its chirality or chiral vector. The chirality is an adapted concept uniquely of each type of nanotube that determines its properties and diameter [25]. The chirality is represented with a pair of indices (n,m) called the chiral vector, which is shown in Fig 1.4. The chiral vector traces the CNT around its circumference from one carbon atom (called the reference point) back to itself. It is expressed as,

2

1 *ma*

*a*
*n*

*C*v* _{h}* = v + v , (1.1)

where *av*_{1} and *av*_{2}are the unit vectors for the graphene hexagonal structure and (n,m) are
integers that represent the number of hexagons away from the reference point to the
point, which will overlap to the reference point after rolled over, in the a1 and a2
directions, respectively.

Using n, m indices CNTs can be classified in three groups: armchair nanotubes
for n = m, zigzag nanotubes for m = 0 or n = 0, and chiral nanotubes for any other
combination. Furthermore, integers n, m also determine whether a CNT is metallic or
*semiconducting, when n – m = 3l (l is an integer), the nanotube is metallic, and when n – *
*m ≠ 3l, the nanotube is semiconducting. The energy gap of the semiconducting CNT *
depends on its diameter and is described as follows [25],

*d*
*a*
*V*

*E _{gap}* =2

_{pp}_{π}

_{c}_{−}

*/ , (1.2)*

_{c}where Vppπ is Slater–Koster π tight-binding matrix element which is one of the Slater–
Koster parameters for sp3 tight-binding, ac-c is the nearest neighbor distance between C-C
bonds (0.142 nm) and d is the diameter of the CNT, which can be calculated using the
following equation [25, 32, 33],
π
2
2
3*a* *n* *mn* *m*
*d* = _{c}_{−}* _{c}* + + (1.3)

**1.4.1 Electronic Band Structure **

**A. Crystal Lattice and Reciprocal Lattice **

Lattice is used to describe arrangement of atoms or molecules in a crystalline liquid or solid. The primitive cell of a carbon nanotube lattice can be described from the unit vectors [22]:

### (

*x*

*y*

### )

*a*

*a*

### (

*x*

*y*

### )

*a*

*a*3ˆ ˆ 2 and ˆ ˆ 3 2 2 1 = + v = − v

_{, (1.4) }

where *av*_{1} and *av*_{2} are the unit cell vectors and a is the lattice constant, a = 3ac-c.

The reciprocal lattice is a lattice in the Fourier space associated with the crystal
lattice. The reciprocal lattice vectors, *b*v_{1} and *b*v_{2} are given as follows [22, 34]:

Figure 1.4: Schematic representation of a chiral vector in the crystal lattice of a carbon nanotube.

Figure 1.5 shows plots of the crystal lattice structure and reciprocal lattice structure for a carbon nanotube with a chiral vector (4,3) generated using MATLAB from the chiral vector and the unit vectors from Eqs. (1.4) and (1.5).

**B. Energy dispersion relation **

The energy dispersion relation defines relationship between the energy, E and wave vector, k. The energy dispersion relation for carbon nanotubes can be calculated from the electronic structure of graphene. The energy dispersion relation of a two-dimensional graphene is given by [35-37],

### (

### )

### [

### ]

### {

### }

12 2 1 2 12 (*k*) *V* 3 2cos(*k* *a* ) 2cos(*k* *a* ) 2cos*k* *a* *a*

*E* * _{D}* v =±

_{pp}_{π}+ v⋅v + v⋅v + v⋅ v −v , (1.6)

where *k*v is the wave vector.

One-dimensional (1D) energy band can be derived from Eq. (1.6) for single-walled carbon nanotubes (SWCNTs) as follows [22, 25, 34],

2
1
2
1
2
cos
4
)
2
cos(
)
2
3
cos(
4
1
)
(
⎪⎭
⎪
⎬
⎫
⎪⎩
⎪
⎨
⎧
⎟⎟
⎠
⎞
⎜⎜
⎝
⎛
+
+
±
= *V* *k* *a* *k* *a* *k* *a*
*k*
*E* *x* *y* *y*
*pp*
*D* π , (1.7)

where the wave vectors kx and ky are obtained using the following relation,

### (

### )

*q*

*N*

*T*

*k*

*T*

*K*

*q*

*K*

*K*

*k*

*k*

*k*

*k*

*,*

_{x}

_{y}_{1}for and 1, , 2 2 K v v v

_{−}

_{<}

_{<}

_{=}⎟ ⎟ ⎠ ⎞ ⎜ ⎜ ⎝ ⎛ + = π π , (1.8)

where k is the magnitude of the wave vector along the nanotube axis, |T| is the magnitude of the translational vector and N is the number of hexagons within a unit cell. |T| and N are given by [22, 25],

### (

### )

*t*

*d*

*m*

*nm*

*n*

*N*

*d*

*d*

*T*2 2 2 , 3

_{=}+ + =

### π

(1.9)Figure 1.5: Schematic representation of (a) crystal lattice and (b) reciprocal lattice of a carbon nanotube with chiral vector (4,3).

where dR is the greatest common divisor of (2n+m) and (2m+n) and dt is the diameter of
the CNT. *K*v_{1} and *K*v_{2} denote the allowed reciprocal wave vectors along the tube and
circumference axis given by [22, 34],

### (

### )

### (

### )

*N*

*b*

*n*

*b*

*m*

*K*

*Nd*

*b*

*m*

*n*

*b*

*m*

*n*

*K*

*R*2 1 2 2 1 1 , 2 2 v v v v v v − = + + + = (1.10)

Figure 1.6 shows the plot of wave vector in k-space (momentum space) for a CNT with chiral vectors (a) (4,2) and (b) (8,2). The reciprocal Bravais lattices are lines, which mean that carbon nanotube is a 1D material. Unlike CNT (4,2), the wave vector of CNT (8,2) passes through K point in the 2D Brillouin zone of graphene. Figure 1.7 shows the plot of the energy band diagram in k-space for a CNT with chiral vectors (a) (4,2) and (b) (8,2).

**1.4.2 Density of States **

The k-vectors in momentum (k) space depend on vectors K1 and K2 as shown in Fig. 1.6. It also represents the area in the momentum space for each state (each single line), which is Ap1-state = ħ2|K1||K2|/2 and a differential area as dAp = ħ2|K1|dk, where dk is in the direction of K2 and ћ is the Planck Constant (h) divided by 2π. The density of states per unit energy is obtained as follows [38-40],

*dE*
*dk*
*dE*
*T*
*dE*
*dE*
*dk*
*K*
*K*
*K*
*A*
*dA*
*dE*
*E*
*D* _{state}*p*
*p*
1
1
2
2
1
2
1
2
4
2
)
(
−
− ⎟
⎠
⎞
⎜
⎝
⎛
=
=
=
π
h
h (1.11)

A combination of Eq. (1.7) for 1D energy dispersion and Eq. (1.11) for density of states can be used to plot the density of states for any chiral vector of carbon nanotube. Figure 1.8 shows density of states plots for a CNT (4,2) and CNT (8,2) abtained from MATLAB. Each peak in Fig. 1.8 is called a Van Hove Singularity and its respective energy represents a conduction energy-band minimum value. The total number of Van Hove Singularities is the number of bands a CNT has. There is a band gap in Fig. 1.8 (a), which means the CNT (4,2) is semiconducting and there is a finite value of the density of

Figure 1.6: Plot of the allowed wave vectors in k-space for a CNT with (a) chiral vector (4,2) and (b) chiral vector (8,2).

Figure 1.8: Plot of the density of states for a CNT with (a) chiral vector (4,2) and (b) chiral vector (8,2).

It is shown from Figs. 1.6, 1.7 and 1.8 that the wave vectors of CNT (4,2) do not pass through K point in the 2D Brillouin zone of graphene, there is a band gap and thereis no state in the band gap. Therefore, CNT (4,2) is a semiconductor. Some of the wave vectors of CNT (8,2) pass through K point in the 2D Brillouin zone of graphene, there is no band gap and there is a finite state in the band gap. Therefore, CNT (4,2) is metallic.

**1.5 Applications of CNTs in Integrated Circuits **

Whereas semiconducting CNTs found applications in making CNT-FETs, metallic CNTs have distinct advantages compared with metal wires for interconnection in integrated circuits.

**1.5.1 Applications of Semiconducting Carbon Nanotubes **

Studies have demonstrated that semiconducting CNTs have excellent electrical properties, including long mean free path (~0.7µm) and high electron mobility [28, 41, 42]. Experiments with CNT-FETs [7, 15, 43] have further demonstrated that transistors based on semiconducting CNTs have large transconductance, which indicates a great potential for sub-nm integrated circuits as demonstrated through the fabrication of five-stage ring oscillator circuit by Chen et. al. [44].

It has been suggested that high-κ dielectrics are essential for future transistors due to low leakage currents and reduced power dissipation [45-47]. However, a fundamental problem for conventional semiconductors is the degradation of electrical properties due to carrier scattering mechanisms introduced at the high-κ film semiconductor interface [48]. Recently, Javey et al. [49-52] have shown that CNT-FETs can be operated in ballistic range with high-κ dielectrics, thereby opening the door to ultrafast devices since both the ballistic transport of electrons and high-κ dielectrics facilitate high on-current that is directly proportional to the speed of a transistor.

Early CNT-FETs were fabricated on oxidized Si substrates [7, 53]. The poor gate coupling due to the thick SiO2 layer and back gate geometry limited their applications.

FETs and p-type CNT-FETs were made [52] and demonstrated for performance similar to current MOSFETs. Additional improvements in the metal-CNT contact resistance at the source and drain ends have led improved CNT-FET performances [51, 54]. Now with improved processing techniques, CNT-FETs with very high ON/OFF switching ratio and high carrier mobility have been fabricated [55-59]. In addition, fabrication of inverters which are composed of n-type and p-type CNT-FETs were also reported in [60, 61]. Recently, Zhang et al. [62] proposed a doping-free fabrication of CNT-based ballistic complementary metal-oxide semiconductor (CMOS) devices and circuits, which are compatible with current CMOS fabrication processes. This work may lead to the fabrication of complex CNT-based integrated circuits.

**1.5.2 Applications of Metallic Carbon Nanotubes **

Metallic CNTs have attracted significant attention because their current carrying
ability is remarkable. Ballistic transport of electrons has been observed and values for the
conductance that approaches the theoretical limit (4e2/h)* [28] have been measured at
small biases [63]. Metallic CNTs hold promise as interconnects in sub-nm CMOS circuits
because of their low resistance and strong mechanical properties. An emerging problem
with interconnects in sub-nm CMOS technology is the breakdown of copper wires due to
electromigration when current densities exceed 106_{ A/cm}2_{ [64]. Preliminary work [65, }
66] have shown that an array of nanotubes can be integrated with silicon technology and
holds promise as vertical vias to carry more than an order of magnitude larger current
densities than conventional vias. Wei et al. [9] have demonstrated that MWCNTs can
carry current densities approaching 1010 A/cm2. Metallic CNTs are excellent wires, with
near-perfect experimentally measured conductance. This is because surface scattering,
disorder, defects and phonon scattering, which lead to a decrease in conductance, have
negligible effects in metallic CNTs, especially when the size of the conductor is
shrinking. The reasons for this are the following.

The acoustic phonon mean free paths in CNTs are longer than a micron [67]. The

dominant scattering mechanisms are due to zone boundary and optical phonons with energies of approximately 160 and 200 meV; but scattering with these phonons at room temperature is ineffective at small biases [68].

In a silicon field effect transistor, there is significant scattering of electrons due to the disordered nature of the Si–SiO2 interface. However, the CNT has a crystalline surface without disordered boundaries [68].

Any potential that is long-ranged compared with the CNT lattice constant will not effectively couple the two crossing sub-bands because of lack of wave vector components in the reciprocal space [69].

The electrons in the crossing sub-bands of carbon nanotubes have a large velocity of 8×105 m/s at the Fermi energy. There are only two sub-bands at the Fermi energy. These two facts make the electron reflection probability due to disorder and defects small [36, 69].

**1.6 Synthesis of Carbon Nanotubes **

At present carbon nanotubes are being synthesized using the following techniques: arc discharge, laser ablation, high-pressure carbon monoxide (HiPCO) and chemical vapor deposition (CVD) methods.

Arc discharge [70], laser ablation [71] and chemical vapor deposition (CVD) [72] are popular methods to produce CNTs. Arc discharge method creates CNTs through arc vaporization of two carbon rods placed end to end, separated by a small gap (~mm), in an enclosure that is usually filled with inert gas at low pressure. In this method, carbon nanotubes are produced at the cathode crater [70]. Laser ablation can be carried out in a horizontal flow tube under a flow of inert gas at controlled pressure. In this set-up, the flow tube is heated to ~1200°C by a tube furnace. Laser pulses enter the tube and strike a target consisting of a mixture of graphite and a metal catalyst such as Co, Pt, Ni, Cu, etc.

processes, which are more suitable for laboratory research. Chemical vapor deposition (CVD) has become the most important commercial approach for synthesis of CNTs. It is also suitable to produce on-chip nanotubes directly, which provides a convenient way for further device fabrication [73]. First, the gaseous carbon molecules, such as methane, carbon monoxide are heated in a furnace and break into atomic carbons [74]. Then the atomic carbons diffuse toward the substrate coated with catalyst particles forming carbon nanotubes. Carbon nanotube synthesis by CVD is essentially a two-step process. The first step is a preparation of patterned catalyst, such as clusters of Ni, Fe and Co. The next step is a synthesis of the nanotube by heating up the substrate in a carbon rich gaseous environment. In all of these methods, the generation of free carbon atoms and the precipitation of dissolved carbon from catalyst particles are involved [25]. The growth terminates when the catalyst particle gets poisoned by the impurities or the stable metal carbide is formed.

Besides these three popular methods, there are other proposed methods to synthesize CNTs, such as flame synthesis, CoMoCat method and high pressure carbon monoxide (HiPCO). Recent work has shown that flame synthesis is an inexpensive large-scale method to produce single-walled carbon nanotubes [75, 76]. In a flame synthesis process, the hydrocarbon fuel combusts to generate enough heat to trigger the process, and to form small aerosol metal catalyst islands. Single-walled carbon nanotubes grow in these catalyst islands in the same way as in the arc discharge and laser ablation processes [77, 78].

CoMoCat method produces SWCNTs of high quality at very high selectivity and with a remarkably narrow distribution of tube diameters. The technique is based on a unique Co-Mo catalyst formulation that inhibits the formation of undesired forms of carbon. During the reaction, cobalt (Co) is progressively reduced from the oxidic state to the metallic form. The strategy used in the CoMoCAT method is to keep the active cobalt stabilized in a non-metallic state by interaction with molybdenum oxide (MoO3). When exposed to carbon monoxide, the Co-Mo dual oxide is carburized, producing molybdenum carbide (Mo2C) and small metallic Co clusters, which remain in a high state of dispersion and result in high selectivity towards SWCNT of very small diameter [79].

This catalytic synthesis of SWCNTs uses a continuous-flow gas phase using CO as the carbon source and Fe(CO)5 as the iron-containing catalyst precursor. Single-walled carbon nanotubes are synthesized when the two gases flow through a heated reactor. Diameter of the nanotubes can be roughly selected by controlling the pressure of carbon monoxide (CO). Single-walled carbon nanotubes with 0.7 nm in diameter, which are expected to be the smallest SWCNTs, have been produced by this method [80].

**1.7 CNT Based Circuit Modeling **

As discussed in Section 1.5, CNT-FETs and metallic CNT wires show performance metrics significantly above those of Si MOSFETs and metal interconnect wires, respectively. Liang et al. [81] fabricated SWCNT CNT-FETs in which MWCNTs are used as local interconnects, making a successful first step towards CMOS circuits fabricated entirely from carbon nanotubes. However, studies of individual CNT-FET and CNT wire are not comprehensive enough to enable conclusions about development of large-scale CNT based integrated circuits. The viability of CNT-FET circuits depends on the behavior of logic gates that are composed of multiple CNT-FETs and used in larger scale circuits. Therefore, circuit models including device models and interconnects model are necessary to predict the behavior of CNT based circuits. Furthermore, like the great help by the CMOS models in optimization of CMOS circuits design, it will be helpful to optimize the CNT based circuits design by utilizing the CNT-FET and CNT interconnect models. As a result, CNT-FET modeling and CNT interconnects modeling are the current focus of most active research in CNT based integrated circuits design.

**1.7.1 CNT-FET Modeling **

A good amount of work on modeling carbon nanotube field-effect transistors (CNT-FETs) has been reported [10, 15, 51, 53, 82-90]. However, these models are still numerical-based and require a mathematical/software realization. Recently, Srivastava et al. [91] have obtained an analytical solution of current transport model for the CNT-FET for analysis and design of CNT-FET based integrated circuits.

**1.7.2 CNT Interconnect Modeling **

A model describing the electromagnetic field propagation along a CNT is indispensable in order to study the interconnection performance of CNT while comparing with traditional metal interconnects. Three theories are used to build different models. Lüttinger liquid theory [92] describes interacting electrons (or other fermions) in one-dimensional conductor and is necessary since the commonly used Fermi liquid model breaks down in one-dimension. Burke [93, 94] regards that electrons are strongly correlated when they transport along the CNT and proposed a transmission line model based on the Lüttinger liquid theory. Another transmission line model was built based on Boltzmann Transport Equation (BTE) [95]. Two-dimensional electron gas, where the charged particles are confined to a plane and neutralized by an inert uniform rigid positive plane background was studied by Fetter [96, 97]. Based on the work of Fetter [96, 97], Maffucci et al. [98] investigated electron transport along the CNT and proposed a third model, fluid model. The first model is based on quantum dynamics concepts; the second model requires solving the Boltzmann Transport Equation; the third model has been developed within the framework of the classical electrodynamics and is simple on concepts and mathematical modeling.

**1.8 Scope of Research **

In this dissertation, we first introduced a channel length modulation parameter, λ in current transport equation for saturation region, which was recently derived by Srivastava et al. [91]. By introducing this parameter, the calculated I-V curve fits the experiments results better. We then derive and analyze the dynamic behavior of CNT-FET based on the current transport equations. We plotted the calculated capacitances for linear and saturation regions of operation of CNT-FET. Thus, we have the models to describe both static and dynamic behaviors of a CNT-FET, which will be discussed in Chapter 2. . In this chapter, we also use Verilog-AMS language to describe the developed non-ballistic CNT-FET models for simulations in Cadence/Spectre and study the CNT based circuits, such as inverter pair, ring oscillator. Furthermore, we have attempted to develop a current transport equation for the ballistic CNT-FETs and shown that computed I-V characteristics are fairly close to experimental I-V characteristics.

In Chapter 3, we make modification in two-dimensional fluid model of electron transport in carbon nanotubes to include electron-electron repulsive interaction and built a semi-classical one-dimensional fluid model. By using this model, we calculate the transmission line parameters for the metallic SWCNT. We also applied the one-dimensional fluid model to study the MWCNT and SWCNT bundle interconnect wires and analyzed their performances in Chapter 4.

The utilization of CNT wires in on-chip inductors is studied in Chapter 5. In Chapters 6 and 7, we introduced some CMOS concepts in CNT based circuits, such as the energy recovery techniques and fault modeling, respectively to study the performances of CNT based circuits.

Conclusion, limitations and future scope for further advancement of research conducted are summarized in Chapter 8.

**CHAPTER 2**

∗
**2 **

**CARBON NANOTUBE FIELD-EFFECT TRANSISTOR **

The field-effect transistor is a type of transistor that relies on an electric field to control the conductivity of a “channel” of one type of charge carrier in a semiconductor material. Devices such as the MOSFET achieve full conduction under the influence of gate voltage when the channel is inverted and current flows between drain and source terminals. The carbon nanotube field-effect transistor (CNT-FET) works under the same principle as the MOSFET. It achieves this operation by using a semiconducting SWCNT as the conducting channel between the source and the drain. The conductivity of the channel depends on the applied gate voltage. For a given gate voltage above a threshold voltage, drain current is obtained by varying the drain to source potential.

**2.1 Background of CNT-FETs **

Rapid development of carbon nanotube field-effect transistor has occurred especially after the first transistors were reported in 1998 by Dekker’s group [7] and others [53]. Such devices used semiconducting silicon substrate (covered by a layer of SiO2) as a back gate and platinum (Pt) electrodes for the drain and source terminals. Carbon nanotubes were produced by laser ablation synthesis [99] and dispersed randomly in the oxidized Si-substrate with contacts for predefined electrodes, resulting in an undefined number of contacts being bridged with CNTs. Consequently, the use of chemical vapor deposition of methane on patterned substrate allowed then the implementation of carbon nanotube growth only in specific catalyst islands. As a result, some of these catalyst metal islands are bridged with CNTs [73].

As mentioned above, early CNT-FETs devices were fabricated on oxidized Si

∗_{ Part of the work is reported in the following publications: }

1. A. Srivastava, J. M. Marulanda, Y. Xu and A. K. Sharma, "Current transport modeling of carbon
*nanotube field effect transistors," physica status solidi (a), vol. 206, no. 7, pp. 1569-1578, 2009. *
2. Y. Xu and A. Srivastava, "Dynamic response of carbon nanotube field effect transistor circuits," in

*Proc. 2009 NSTI Nanotechnology Conference and Expo, Houston, TX, May 3-7, 2009, vol. 1, pp. *

625-628.

3. Y. Xu and A. Srivastava, "Transient behavior of integrated carbon nanotube field effect transistor
*circuits and bio-sensing applications," in Proc. of SPIE: Nano-, Bio, and Info-Tech Sensors and *

substrate, the gate coupling and control of the drain current was very poor due to the thick SiO2 layer and back gate geometry [7, 53]. In 2002, major improvement was observed after the implementation of CNT-FETs using the top-gate geometry [100]. Transconductance of 3.25 μS and subthreshold slope of 130 mV/decade were found, which were much higher than the values in alternate devices [101] with transconductance of only 0.3 μS. Further enhancement in performance was obtained by using high-κ dielectric [52] and electrolyte gating [102, 103]. Javey et al. [52] reported the integration of top gated p-type CNT-FETs using the high-κ dielectric material ZrO2 (k = 25) as the gate oxide, achieving a transconductance and subthreshold slope of 12 μS and 70 mV/decade, respectively. Electrolyte gating, first introduced by Krüger et al. [104], involves applying a voltage at the electrolyte gate which creates an electrochemical potential between the electrolyte and the device. The leakage current between the electrolyte and the electrodes is negligible and the electrolyte behaves as an insulating liquid gate [102]. Subthreshold slopes of 80 mV/decade and hole mobility of 1500 cm2/Vsec were reported by Rosenblatt et al. [102]. Later on, hole mobility of 2600 cm2/Vsec and subthreshold slopes of 62 mV/decade [103], corresponding to a gate efficiency parameter, α = 0.97 (the shift in Fermi level for a change in the gate voltage of ∆Vgb = 1V), which is approaching the ideal efficiency value of 1, were also reported. Recently, Javey et al. [49-52] have shown that CNT-FETs can be operated in ballistic range with high-κ dielectrics, thereby opening the door to ultrafast devices since both the ballistic transport and high-κ dielectrics facilitate high on-current that is directly proportional to the speed of a transistor.

Figure 2.1 shows the typical vertical cross-section of a CNT-FET. According to the types of contact between source/drain metals and the semiconducting CNT, the CNT-FETs can be categorized as: (a) Schottky Barrier CNT-CNT-FETs (SB-CNT-CNT-FETs), with a Schottky contact between metal and semiconducting CNT at source and drain regions, and (b) Repress Barrier CNT-FETs (RB-CNT-FETs), with either decreased Schottky barrier in the contact between metal and semiconducting CNT at source and drain regions

between metal and semiconducting CNT at source and drain regions. Schottky Barrier CNT-FETs [16, 53] show large barriers at the electrode-nanotube interfaces with strong dependence on the height of these barriers. Repress Barrier CNT-FETs [51, 105] show small, negative, or no barrier at the electrode-nanotube interfaces. The second type of transistors allows a device modeling approach similar to current MOSFETs models, so-called MOSFET-like CNT-FETs. This type of CNT-FETs were achieved by either using heavily doped CNT sections as source and drain [105, 106] or using metals with proper work functions to contact the semiconducting SWCNT, for example, scandium (Sc) for n-type CNT-FETs [62] and palladium (Pd) for p-type CNT-FETs [51, 107].

Both of the two CNT-FETs can also be categorized as non-ballistic and ballistic CNT-FETs [7, 15, 28, 41-43, 49-52, 108]. One of the promising properties of CNT-FET is its absence of scattering in the channel, which is ballistic transport. Studies have demonstrated that semiconducting CNTs have excellent electrical properties, including long mean free path (~0.7µm) and high electron mobility [28, 41, 42]. Experiments with CNT-FETs [7, 15, 43] have further demonstrated that transistors based on semiconducting CNTs have large transconductance, which indicates a great potential for sub-nm integrated circuits.

With the advancement in fabrication technology of CNT-FETs, efforts have also been made in modeling of the current transport behavior and models have been developed for the design of CNT-FET based logic circuits [10, 85, 89]. An analytical model has been built by Srivastava et al. [91] to characterize the current transport in CNT-FETs for the analysis and design of integrated circuits. We have used these current transport equations to generate I-V characteristics for CNT-FETs using different chiral vectors (n,m) of carbon nanotubes. In this work, based on the static model of Srivastava et al. [91], we have built a dynamic model to describe the transition behavior of CNT-FETs and using these models we have studied performances of some basic CNT-CNT-FETs circuits, such as the inverter and ring oscillator. In addition, the current equation of ballistic CNT-FET is also studied.

**Figure 2.1: Typical vertical cross-section of a CNT-FET. Note: Insulators in the figure **
are SiO2 or high-κ dielectric.

**2.2 Surface Potential of CNT-FETs **

Figure 2.2 (a) and (b) show the basic cross section of a Schottky Barrier CNT-FET and MOSCNT-FET-like CNT-CNT-FET, respectively, including the charge distributions. Gate oxide and SiO2 are corresponding to the insulators in Fig. 2.1. Both of these two structure can be utilized in realizing non-ballistic and ballistic CNT-FETs [7, 15, 28, 41-43, 49-52, 108] since the necessary and sufficient condition that the carrier transport in a CNT-FET is ballistic is that the length of channel (length of CNT between source and drain) is shorter than the mean free path of carrier in it. Figure 2.2 (c) shows the corresponding potential distributions between the gate and the substrate. In Fig. 2.2 (a) and (b), charge distributions are explained as follows: the charge on the gate is Qg, the charges in the oxide layers are Q01 and Q02, the charge inside the CNT is Qcnt and the charge in the substrate is Qsubs. In Fig. 2.2 (c), six different potential distributions are shown, which are also described as follows: the voltage between the gate and the substrate (back gate) is Vgb, the potential drop across the oxides are ψox1 and ψox2, the surface potential in the substrate with respect to the back gate, ψsubs, the potential across the CNT, ψcnt and the work function difference between the gate and the substrate materials is Фms.

Using Kirchoff’s voltage law, the potential balance and charge neutrality condition, we can write for the Fig. 2.2,

1
2 *cnt* *ox*
*ox*
*subs*
*ms*
*gb*
*V* =φ +ψ +ψ +ψ +ψ (2.1)
0
02
01′ + ′ + ′ + ′ =
+
′ _{cnt}_{subs}*g* *Q* *Q* *Q* *Q*
*Q* (2.2)

The prime in Eq. (2.2) denotes the charge per unit area. фms is divided in two parts and expressed as follows,

*cs*
*mc*

*ms* φ φ

φ = + (2.3)

where фmc and фcs are the work function differences between the metal gate and carbon nanotube materials and the carbon nanotube and substrate materials, respectively.

Figure 2.2: (a) Plot of the charges from the gate to the substrate for Schottky Barrier CNT-FET, (b) Plot of the charges from the gate to the substrate for MOSFET-like CNT-FET and (c) plot of the potential distribution from the gate to the substrate in a CNT-FET [91].

can be re-written as follows,
*s*
*cnt*
*ox*
*mc*
*gb*
*V* =φ +ψ _{1}+ψ _{,} (2.4)

where ψcnt,s describes the surface potential at the interface of the gate oxide and the carbon nanotube with respect to the back gate.

The electric field in terms of the charge distribution can be written from the Maxwell’s third equation [109] and is given by,

### ( )

ε*E*=ρ

*v*

∇ (2.5)

where ε is the permittivity of the material, E is the electric field and ρv is the charge per unit volume. Assuming that the electric field in Fig. 2.2 (a) is constant through the gate oxide region and at the bottom edge of the carbon nanotube, Eq. (2.5) can be integrated between the gate and the bottom edge of the carbon nanotube, that is in Fig. 2.2 (a) from

0 =

*y* to*y*=*Tox*1+*dcnt*, to obtain the following Eq. (2.6), where dcnt is the diameter of the

carbon nanotube. In this derivation, we have assumed that the carbon nanotube has a relative permittivity, εcnt. We can write Eq. (2.6) as follows,

*cnt*
*ox*
*ox*
*cnt*
*cntE* −ε 1*E* 1 =*Q*01′ +*Q*′
ε (2.6)

where Ecnt and Eox1 are the electric fields along the y-axis across the carbon nanotube and gate oxide, respectively.

We assume that any charge applied at the gate is compensated only by an induced charge in the carbon nanotube as follows:

*cnt*

*g* *Q*

*Q*′ =−Δ ′

Δ (2.7)

Furthermore, there is a specific gate voltage, called the flat band voltage, Vfb [110], when applied at the gate with respect to the back gate; it compensates for the band bending at the gate oxide and carbon nanotube interface. Under this flat band condition, the electric field at the bottom edge of the carbon nanotube, Ecnt in Eq. (2.6) can be

neglected. Under this assumption and replacing Eox1 with the potential gradient

### ( )

*dy*

*y*

*d*ψ

*ox1*− in Eq. (2.6) we obtain,

### ( )

*cnt*

*ox*

*ox*

_{dy}*Q*

*Q*

*y*

*d*

_{′}+ ′ =

_{01}1 1 ψ ε (2.8)

By integrating Eq. (2.8) through the gate oxide region, that is in Fig. 2.2(a) from y = 0 to y = Tox1, we can write an expression for the gate oxide potential as:

1
01
1
*ox*
*cnt*
*ox*
*C*
*Q*
*Q*
′
′
+
′
−
=
ψ (2.9)

In Eq. (2.9), Ćox1 is the gate oxide capacitance per unit area. Substituting Eq. (2.9) in Eq. (2.4), we obtain an expression for the gate voltage given by,

1
01
1
,
*ox*
*mc*
*ox*
*cnt*
*s*
*cnt*
*gb*
*C*
*Q*
*C*
*Q*
*V* =ψ − +φ − (2.10)

In Eq. (2.10), Qcnt, Q01 and Cox1 are the total charges and capacitance, respectively, which are obtained by multiplying Q́01, Q́cnt, and Q́02 with their respective areas. Cox1, the capacitance between the gate and the carbon nanotube, can be redefined by considering the carbon nanotube to be a line of charge and the gate to be a planar conducting plate. Therefore, the gate oxide capacitance of thickness Tox1 of a carbon nanotube of length L and radius r can be defined as follows [111],

⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛ _{+} _{+} _{+}
=
*r*
*r*
*T*
*T*
*r*
*T*
*L*
*C*
*ox*
*ox*
*ox*
*ox*
*ox*
1
2
1
1
1
1
2
ln
2πε
(2.11)

In Eq. (2.10), the flat band voltage, Vfb is:

The gate voltage, Vgb in Eq. (2.10) after combining with the Eq. (2.12) can be
expressed as follows,
*fb*
*ox*
*cnt*
*s*
*cnt*
*gb* *V*
*C*
*Q*
*V* = − +
1
,
ψ (2.13)

In Eq. (2.13), ψcnt,s can be explained as a control potential in the carbon nanotube in charge of shifting the energy band at the interface of the gate oxide and carbon nanotube.

In Eq. (2.13), the charge inside the carbon nanotube can be calculated using the relation |Qcnt| = qncntL, where ncnt is the carrier concentration per unit length inside the carbon nanotube, which was derived in [112] and is given by,

### ( )

### (

### )

### (

### )

### ∫

∞_{−}− + + + = 0 1 1 2 3 8

*dx*

*e*

*E*

*kTx*

*x*

*E*

*kTx*

*a*

*V*

*kT*

*n*

*x*

*c*

*c*

*pp*

*cnt*η π π η (2.14)

where a is the lattice constant, Vppπ is Slater–Koster π tight-binding matrix element which is one of the Slater–Koster parameters for sp3 tight-binding, k is Boltzmann’s constant and T is the temperature. The parameter, η is given by:

*kT*
*E*
*E _{F}* −

*=*

_{c}η (2.15)

where Ec is the conduction band minima.

Under two limiting cases, the charge inside the carbon nanotube can be described
as in [112],
Limit 1, η << –1:
*kT*
*E*
*E*
*c*
*cnt*
*c*
*F*
*e*
*I*
*N*
*qL*
*Q*
−
= , (2.16)
Limit 2, η >> 1:

*kT*
*E*
*E*
*N*
*L*
*q*
*Q* *F* *c*
*c*
*cnt*
2
2_{−}
= , (2.17)
where

### (

### )

### [

### {

### ( )

### ( )

### ( )

### ( )

### ( )

### ]

### ( )

### [

### ( )

### ]

### [

### ]

### }

1 2 2 8 5 2 2 1 2 2 1 6 1 2 6 1 2 2 1 2 2 1 2 485 2 241 3 241 3 6 1 3 165 2 4 1 2 2 1 2 1 2 2 1 2 1 6 1 6 int 0 2 6 1 2 1 2 1 2 ln 1 1 2 + = = = − + + + − − + + + + − + + + − + − + + + − + + + − − + + + − + =### ∑

*A*

*x*

*A*

*x*

*c*

*kT*

*E*

*kT*

*Ec*

*kT*

*Ec*

*kT*

*E*

*kT*

*E*

*kT*

*E*

*kT*

*E*

*kT*

*Ec*

*kT*

*Ec*

*kT*

*Ec*

*kT*

*E*

*kT*

*E*

*kT*

*E*

*kT*

*E*

*A*

*kT*

*E*

*kT*

*E*

*A*

*xE*

*kTx*

*kT*

*A*

*A*

*A*

*x*

*A*

*Ax*

*A*

*A*

*x*

*x*

*x*

*A*

*x*

*A*

*A*

*A*

*Ax*

*x*

*x*

*A*

*x*

*x*

*x*

*e*

*I*

*c*

*c*

*c*

*c*

*c*

*c*

*c*

*c*

*c*

*kTc*

*E*

*c*

*c*and

*a*

*V*

*kT*

*N*

*pp*

*c*π π 3 8 = .

In order to effectively describe the potential inside the carbon nanotube, we need to determine the energy separation between the Fermi level and the conduction band at the interface of the gate oxide and carbon nanotube. Assuming a flat band energy level in the carbon nanotube, we can say that the Fermi level and the conduction band at the interface of the gate oxide and carbon nanotube will be shifted by an amount determined by qVcb and qψcnt,s, respectively; where Vcb is the induced potential between the carbon nanotube and the substrate due to the drain and source terminal voltages. The potential, Vcb varies from Vsb (source to back gate potential) to Vdb (drain to back gate potential). Figure 2.3 shows the energy band diagram from gate to substrate of a CNT-FET when (a) Vgb = |Vfb| and (b) Vgb > 0 [91]. In Fig. 2.3(a), we have used hafnium dioxide (HfO2) as the gate oxide, which is a high-κ dielectric insulator material. Furthermore, ф0 in Fig. 2.3(a) is the carbon nanotube surface potential, ψcnt,s when Vgb = Vfb and ψcnt = 0. ф0 is then given by,

*cs*
*subs*

*ox* ψ φ

ψ

As it was previously done, by integrating Eq. (2.5) from y = Tox1+dcnt to y = Tox1+dcnt+Tox2+dsubs, where dsubs is the thickness of Qsubs in the substrate as shown in Fig. 2.2(a), we can write,

*subs*
*ox*
*ox*
*s*
*sE* −ε 2*E* 2 =*Q*02′ +*Q*′
ε (2.19)

where εs is the permittivity of the substrate material. Assuming the electric field, Es is to be negligible deep inside the substrate and replacing Eox2 with the potential gradient

### ( )

*dy*

*y*

*d*ψ

*ox 2*− in Eq. (2.19), we obtain,

### ( )

*subs*

*ox*

*ox*

*Q*

*Q*

*dy*

*y*

*d*′ + ′ =

_{02}2 2 ψ ε (2.20)

By integrating Eq. (2.20) from y = Tox1+dcnt to y = Tox1+dcnt+Tox2 in Fig. 2.2(a) we can obtain an expression for the second oxide potential as:

2
02
2
*ox*
*subs*
*ox*
*C*
*Q*
*Q*
′
′
+
′
−
=
ψ (2.21)

The total capacitance Cox2, which is the capacitance between the carbon nanotube and the substrate and can be obtained as follows [111]:

⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛ _{+} _{+} _{+}
=
*r*
*r*
*T*
*T*
*r*
*T*
*L*
*C*
*ox*
*ox*
*ox*
*ox*
*ox*
2
2
2
2
2
2
2
ln
2πε
(2.22)

Assuming Qsubs and ψsubs to be small compared to Q02 and фcs + ψox2, we can rewrite Eq. (2.18) for ф0 as follows:

2
02
0
*ox*
*cs*
*C*
*Q*
−
=φ
φ (2.23)

We are interested in the separation between the Fermi level and conduction band at the interface of the gate oxide and carbon nanotube. Following the Fig. 2.3(a) we can

**E _{Fsurf} - E_{Csurf}= E_{F} - qV_{cb}**

**+q**ψ

**cnt,s - q**φ

**0- EC**

**(a)**

**EVAC**

**EC**

**E**

_{Fm}

_{E}**C**

**E**

_{C}**E**

_{V}**EV**

**EV**

**Aluminium** **HfO2** **CNT** **SiO2** **p+ - Substrate**
**EC**
**E _{V}**

**q**ψ

**cnt,s=q**φ

**0**

**qV**

_{gb}= qV_{fb}**EVAC**

**q**φ

**0**

**(b)**

**E**

_{VAC}

_{E}**C**

**EFm**

**EC**

**E**

_{C}**E**

_{V}**EV**

**EV**

**Aluminium** **HfO2** **CNT** **SiO2** **p+ - Substrate**

**E _{C}**

**EV**

**E**

_{VAC}**qV**

_{gb}**q**ψ

**cnt,s**

**qVcb**

**EF**

**EE**

_{Fsurf}Csurf**q**ψ

**cnt**

**EF**

**E**

_{F}observe that the conduction band of the carbon nanotube is shifted by an amount of ψcnt,s – ф0 which can be expressed through the following relation [110, 113],

### (

ψ , −φ0### )

−
= _{c}_{cnt}_{s}*Csurf* *E* *q*

*E* (2.24)

where ECsurf is the conduction band energy at the interface of the gate oxide and carbon nanotube. The Fermi level at the interface, EFsurf is shifted by an amount of Vcb and is

expressed as follows [110, 113],

*cb*
*F*

*Fsurf* *E* *qV*

*E* = − (2.25)

From Eqs. (2.24) and (2.25) we can write following equation for intrinsic CNT:

### (

*cnts*

*cb*

### )

*c*

*F*

*Csurf*

*Fsurf* *E* *E* *q* *V* *E*

*E* − = + ψ _{,} − −φ_{0} − (2.26)

The shift in the Fermi level of the carbon nanotube due to impurity doping can be
obtained as follows. The carrier concentration in a doped carbon nanotube is given by
[91],
*kT*
*E*
*E*
*c*
*cnt*
*c*
*F*
*e*
*I*
*N*
*n*
−
= (2.27)

The intrinsic carrier concentration, ncnt,i can be obtained by setting EF = 0 in Eq.
(2.27),
*kT*
*E*
*c*
*i*
*cnt*
*c*
*e*
*I*
*N*
*n*
−
=
, (2.28)

Using Eq. (2.28), we can rewrite Eq. (2.27) as follows:

⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
=
*i*
*cnt*
*cnt*
*F*
*n*
*n*
*kT*
*E*
,
ln (2.29)

The carrier concentration in a doped carbon nanotube can also be obtained by adding an ionized impurity doping concentration, N in Eq. (2.28) as follows:

*N*
*n*

*n _{cnt}* =

_{cnt}_{,}

*+ (2.30)*

_{i}The ionized impurity concentration, N in Eq. (2.30) can be either donor atoms, ND or acceptor atoms, NA.

In an intrinsic carbon nanotube, the Fermi level lies in the middle of the band gap; we can use Eq. (2.29) to express the shift in the Fermi level depending upon the doping. Furthermore, using Eq. (2.30) we can define a parameter ∆EF given by,

⎟
⎟
⎠
⎞
⎜
⎜
⎝
⎛
+
±
=
Δ
*i*
*cnt*
*F*
*n*
*N*
*kT*
*E*
,
1
ln (2.31)

where ∆EF is positive for an n-type carbon nanotube (donors impurity concentration, N = ND) and negative for a p-type carbon nanotube (acceptors impurity concentration, N = NA). Equation (2.31) is valid for N ≤ ncnt,i(eEg/2kT-1) and the impurity concentration, N is limited by the maximum value of |∆EF| which can be determined from energy gap of the carbon nanotube as ∆EF ≤ Eg/2. Thus, using Eq. (2.31) for the shift in the Fermi level, we can rewrite Eq. (2.26) for the n-type CNT-FET as follows:

### (

*cnts*

*cb*

### )

*c*

*F*

*Csurf*

*Fsurf* *E* *E* *q* *V* *E*

*E* − =Δ + ψ _{,} − −φ_{0} − (2.32)

Using Eq. (2.32) in the analytical expressions for the charge inside the carbon nanotube given by Eqs. (2.16) and (2.17), the gate substrate voltage, Vgb, in Eq. (2.10) can be rewritten as:

### (

*cnts*

*cb*

### )

*fb*

*s*

*cnt*

*gb*

*f*

*V*

*V*

*V*=ψ , −δ ψ , , + (2.33) where

### (

### )

( )### (

### )

⎪⎪ ⎪ ⎪ ⎨ ⎧ − − − + Δ − + − + ≤ = − − − + Δ*E*

*q*

*qV*

*q*

*E*

*q*

*KT*

*q*

*E*

*q*

*ΔE*

*φ*

*V*

*ψ*

*for*

*Ie*

*V*

*f*

*F*

*cnt*

*s*

*cb*

*c*

*c*

*F*

*0*

*cb*

*,s*

*cnt*

*kT*

*E*

*V*

*q*

*EF*

*cnts*

*cb*

*c*2 2 0 , ; ; , 0 , φ ψ ψ φ ψ